A reproducible, high throughput method for fabricating fibrin gels
© Murphy and Leach; licensee BioMed Central Ltd. 2012
Received: 21 June 2012
Accepted: 31 July 2012
Published: 8 August 2012
Fibrin gels are a promising biomaterial for tissue engineering. However, current fabrication methods are time intensive with inherent variation. There is a pressing need to develop new and consistent approaches for producing fibrin-based hydrogels for examination.
We developed a high throughput method for creating fibrin gels using molds fabricated from polydimethylsiloxane (PDMS). Fibrin gels were produced by adding solutions of fibrinogen and thrombin to cylindrical defects in a PDMS sheet. Undisturbed gels were collected by removing the sheet, and fibrin gels were characterized. The characteristics of resulting gels were compared to published data by measuring compressive stiffness and osteogenic response of entrapped human mesenchymal stem cells (MSCs). Gels exhibited compressive moduli nearly identical to our previously reported fabrication method. Trends in alkaline phosphatase activity, an early marker of osteogenic differentiation in MSCs, were also consistent with previous data.
These findings demonstrate a streamlined approach to fibrin gel production that drastically reduces the time required to make fibrin gels, while also reducing variability between gel batches. This fabrication technique provides a valuable tool for generating large numbers of gels in a cost-effective manner.
KeywordsFibrin Hydrogel Polydimethylsiloxane Mesenchymal stem cells Bone
Fibrin gels are a promising biomaterial, as they can be delivered in a minimally invasive manner or formed into an implant and tuned to possess desired characteristics (e.g., gelation rate, compressive stiffness, degradation rate, etc.) [1–3]. These biodegradable hydrogels are produced through the combination of proteins found in the body, fibrinogen and thrombin, which generates a provisional matrix that allows cells to encounter an environment that closely mimics the ECM of a damaged tissue [4, 5]. A wide variety of methods are available to manipulate the physical properties of these gels, including increasing the protein concentrations , cross linking via enzymes or UV radiation , and adjusting the Ca2+ concentration [8–10]. Recently, we showed that supplementing the pre-gel solution with various concentrations of sodium chloride (NaCl) alters gel stiffness . This approach addresses many shortcomings of other fibrin gel fabrication techniques; namely, that one can manipulate gel stiffness using biomimetic concentrations of fibrinogen and thrombin while maintaining a slow gelation time, thus limiting stress on entrapped cells .
Previous work in our laboratory fabricated fibrin gels by combining solutions of fibrinogen and thrombin in parafilm-covered, cylindrical nylon washers . Once gelation was complete, the gels were carefully removed with a metal spatula and placed in tissue culture plates. This method was taxing to reproduce, required significant preparation, and was time intensive, requiring more than 12 hours, on average, to produce up to 30 gels. Poly-dimethylsiloxane (PDMS) is a chemically inert, hydrophobic, silicone-based organic polymer that can be produced with a wide range of viscosities. High viscosity PDMS is often used in microfluidic devices, and while pliable, it will retain its form indefinitely. These properties make PDMS an ideal material for creating a non-fouling, biologically inert substrate for use in fabricating fibrin gels [13, 14].
This study demonstrates a novel method for producing fibrin gels using a PDMS mold. Compared to previous methods, these gels can be fabricated in a high throughput and cost-effective manner, thus providing an improved technique for generating reproducible substrates for use in studies of materials science, cellular biology, and tissue development.
Fabrication of PDMS mold
Cylindrical molds were formed using a 6 mm diameter biopsy punch (Accuderm Inc., Ft. Lauderdale, FL, USA) pressed into a 2 mm thick sheet of PDMS (Dow Corning, Midland, MI, USA). The PDMS mold can be used for up to six months. To initiate gel fabrication, the PDMS mold was rinsed with distilled water, sterilized by immersion in 70% ethanol for up to 2 min, and allowed to dry in an aseptic environment for 5 min. When dry, the PDMS sheet was placed in a non-treated sterile polystyrene dish, creating a seal.
Fibrin gel preparation
Compressive testing of fibrin gels
We measured the compressive moduli of gels made with varying salt concentrations to verify that fibrin gels fabricated in this manner possessed comparable mechanical properties to those prepared using previously published methods. Acellular gels containing increasing NaCl content were allowed to gel for 1 hr, transferred to PBS and allowed to swell for 1 hr, and then any excess fluid was blotted off before analysis. Gels were then loaded between two flat platens and compressed at 1 mm/min (Instron 3345 Compressive Testing System, Norwood, MA, USA). The compressive moduli were measured from the 0-5% linear regions of the stress–strain graphs .
Cell culture and osteogenic response
We analyzed the osteogenic response of human mesenchymal stem cells (MSCs) entrapped within fibrin gels as a measure of comparison with previously reported fabrication methods. Human MSCs (Lonza, Walkersville, MD, USA) were expanded in αMEM (Invitrogen, Carlsbad, CA, USA) supplemented with 10% fetal bovine serum (JR Scientific, Woodland, CA, USA) and 1% penicillin/ streptomycin (Mediatech, Manassas, VA, USA) until use at passage 6. MSCs were added to the pre-gel solution at 1.5 × 10  cells mL-1 of gel solution and cultured for various time intervals in the αMEM media described above.
At days 3, 5, 7, and 10, the gels were collected and sonicated in 400 μL passive lysis buffer (Promega, Madison, WI). Samples were centrifuged at 5000 rpm for 10 min to pellet the cell debris, and the supernatant was collected. The supernatant was analyzed for intracellular alkaline phosphatase (ALP) activity using a p-nitrophenyl phosphate (PNPP) colorometric assay as previously described . DNA content, a measure of cell growth, was assayed from the supernatant using the Quant-iT PicoGreen dsDNA Assay Kit (Invitrogen).
Results are expressed as mean ± standard deviation (SD). Statistical analyses were performed by ANOVA followed by Student–Newman–Keuls post-hoc tests assessing significance to probability values (p) <0.05.
Results and discussion
Comparison of compressive stiffness between two fabrication methods
St Dev (kPa)
St Dev (kPa)
Osteogenic response of entrapped MSCs
We developed a reproducible, cost-effective, and quick method for fabricating fibrin gels using molds formed in PDMS. This new fabrication method generated fibrin gels with similar compressive moduli and the capacity to promote osteogenic differentiation of entrapped MSCs. Values from these two characterization assays were similar to our previous data, thus validating this new approach for the consistent and reproducible production of many hydrogels in a fraction of the time required for previous methods.
This work was supported by the NIH Grants R03-DE021704 and R21-AG036963 and the AO Foundation (C10-39 L) to JKL.
- Janmey P, Winer JP, Weisel JW: Fibrin gels and their clinical and bioengineering applications. J R Soc Interface. 2009, 6: 1-10. 10.1098/rsif.2008.0327.PubMedPubMed CentralView ArticleGoogle Scholar
- Shaikh FM, Callanan A, Kavanagh EG, Burke PE, Grace PA, McGloughlin TM: Fibrin: a natural biodegradable scaffold in vascular tissue engineering. Cells Tissues Organs. 2008, 188: 333-346. 10.1159/000139772.PubMedView ArticleGoogle Scholar
- Barsotti M, et al: Fibrin acts as biomimetic niche inducing both differentiation and stem cell marker expression of early human endothelial progenitor cells. Cell Prolif. 2011, 44: 33-48. 10.1111/j.1365-2184.2010.00715.x.PubMedView ArticleGoogle Scholar
- Hubbell JA: Biomaterials in tissue engineering. Nat Biotechnol. 1995, 13: 565-576. 10.1038/nbt0695-565.View ArticleGoogle Scholar
- Grassl ED, Oegema TR, Tranquillo RT: Fibrin as an alternative biopolymer to type-1 collagen for the fabrication of a media equivalent. J Biomed Mater Res. 2002, 60: 607-612. 10.1002/jbm.10107.PubMedView ArticleGoogle Scholar
- Bensaïd W, Triffitt JT, Blanchat C, Oudina K, Sedel L, Petite H: A biodegradable fibrin scaffold for mesenchymal stem cell transplantation. Biomaterials. 2003, 24: 2497-2502. 10.1016/S0142-9612(02)00618-X.PubMedView ArticleGoogle Scholar
- Siebenlist KR, Mosesson MW: Progressive cross-linking of fibrin gamma chains increases resistance to fibrinolysis. J Biol Chem. 1994, 269: 28414-28419.PubMedGoogle Scholar
- Blombäck B, Bark N: Fibrinopeptides and fibrin gel structure. Biophys Chem. 2004, 112: 147-151. 10.1016/j.bpc.2004.07.013.PubMedView ArticleGoogle Scholar
- Carr ME, Gabriel DA, McDonagh J: Influence of Ca2+ on the structure of reptilase-derived and thrombin-derived fibrin gels. Biochem J. 1986, 239: 513-516.PubMedPubMed CentralView ArticleGoogle Scholar
- Okada M, Blomback B: Calcium and fibrin gel structure. Thromb Res. 1983, 29: 269-280. 10.1016/0049-3848(83)90039-7.PubMedView ArticleGoogle Scholar
- Davis HE, Miller SL, Case EM, Leach JK: Supplementation of fibrin gels with sodium chloride enhances physical properties and ensuing osteogenic response. Acta Biomater. 2011, 7: 691-699. 10.1016/j.actbio.2010.09.007.PubMedView ArticleGoogle Scholar
- Zhao HG, Ma L, Zhou J, Mao ZW, Gao CY, Shen JC: Fabrication and physical and biological properties of fibrin gel derived from human plasma. Biomed Mater. 2008, 3: 15001-15010. 10.1088/1748-6041/3/1/015001.View ArticleGoogle Scholar
- Marois Y, Be MC: Studies of primary reference materials low-density polyethylene and polydimethylsiloxane : A review. J Biomed Mater Res. 2001, 58: 467-477. 10.1002/jbm.1043.PubMedView ArticleGoogle Scholar
- Regehr KJ, et al: Biological implications of polydimethylsiloxane-based microfluidic cell culture. Lab Chip. 2009, 9: 2132-2139. 10.1039/b903043c.PubMedPubMed CentralView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.